Memory effects in annealed hybrid gold nanoparticles/block copolymer bilayers
© Torrisi et al; licensee Springer. 2011
Received: 6 September 2010
Accepted: 23 February 2011
Published: 23 February 2011
We report on the use of the self-organization process of sputtered gold nanoparticles on a self-assembled block copolymer film deposited by horizontal precipitation Langmuir-Blodgett (HP-LB) method. The morphology and the phase-separation of a film of poly-n-butylacrylate-block-polyacrylic acid (Pn BuA-b-PAA) were studied at the nanometric scale by using atomic force microscopy (AFM) and Time of Flight Secondary Ion Mass Spectrometry (TOF-SIMS). The templating capability of the Pn BuA-b-PAA phase-separated film was studied by sputtering gold nanoparticles (NPs), forming a film of nanometric thickness. The effect of the polymer chain mobility onto the organization of gold nanoparticle layer was assessed by heating the obtained hybrid Pn BuA-b-PAA/Au NPs bilayer at T >T g. The nanoparticles' distribution onto the different copolymer domains was found strongly affected by the annealing treatment, showing a peculiar memory effect, which modifies the AFM phase response of the Au NPs layer onto the polar domains, without affecting their surfacial composition. The effect is discussed in terms of the peculiar morphological features induced by enhanced mobility of polymer chains on the Au NPs layer.
Recent advances in the patterning of polymers have enabled the fabrication of integrated micro- and nanosystems with high degree of complexity and functionality. For example, block copolymers have attracted immense interest for nanotechnology applications because of easy processability and low-cost fabrications. The chemically distinct and immiscible polymer blocks in block copolymers microphase-separate and self-assemble into ordered patterns on the scale of nanometers [1–3]. This soft nanostructured polymer film can further be used as a template for patterning of hard inorganic materials such as metal nanoparticles [4–10]. Metal nanoclusters in a matrix of insulating polymer have unique physical properties and have been proposed for optical, electrical and magnetic applications [11–14].
Previous studies demonstrate that metal nanoparticles can preferentially decorate a particular domain in a diblock copolymer film. In general, the specific nature of the selective gold-polymer interaction that causes the self-assembly is still far from being completely understood.
Patterning of metal nanoparticles within polymer films has been achieved using four main routes. The first method is vapour phase co-deposition of polymers/nanoparticles in high vacuum followed by thermal annealing [15–18]. Annealing of the polymer film above the glass transition temperature (T g) of the polymer allows structural relaxation of the polymer matrix and was proven to be responsible for the dispersion of the metal nanoparticles within the polymer film. The second method is based on the deposition from a mixture of block copolymer and organic-coated nanoparticles in solution onto a solid surface followed by the annealing step [19–25]. The third method employs the dewetting of polymer films made from low concentrations of mixed solutions of polymer and polymer-grafted nanoparticles to create metal nanostructures [26–29]. The fourth method uses the self-organization characteristic of evaporated nanoparticles on a self-assembled polymer film to create nanopatterning by selective adsorption .
We used the sputtering technique to investigate the deposition behaviour of gold nanoparticles onto block copolymer template.
Substrate cleaning and polymer coating
A silicon wafer 100 (p-type, Boron-doped) was cut into 1 × 1 cm2 pieces. The silicon substrates were cleaned as follows: soaking in the cleaning bath at 75°C for 10 min. The cleaning solution was composed of 100 ml of 96% NH4OH, 35 ml of 35% H2O2 and 65 ml deionized water. The cleaned substrates were further rinsed in deionized water for 10 min and finally deposited by horizontal precipitation Langmuir-Blodgett (HP-LB) method .
A CHCl3 1 mg/ml solution of poly-n-butylacrylate-block-polyacrylic acid (Pn BuA-b-PAA) (MW 13,000 Da) was used for film deposition by means of HP-LB.
This solution was used for preparation of Langmuir polymer layers at the water/air interface in a computer-controlled trough (LT-102, MicrotestMachines, Belarus). The floating film was compressed at a rate of 0.5 mm/s (or 0.75 cm2/s) and the corresponding isotherms were acquired. LB films of each mixture (applied pressure 11-14 mN/m) were transferred on cleaned silicon 100 substrates by means of HP-LB method.
Gold nanoparticles sputtering deposition
The depositions were carried out using an RF (60 Hz) Emitech K550x Sputter coater apparatus onto the substrates and clamped against the cathode located straight opposite of the Au source (99.999% purity target). The electrodes were laid at a distance of 40 mm under Ar flow keeping a pressure of 0.02 mbar in the chamber. The deposition time was 30 s with working current of 10 mA, corresponding to about 3 nm of deposited Au.
The polymer films were annealed in a vacuum oven at 115°C for 15, 30, 45, 60, 90 min.
AFM images were obtained in tapping mode using a MultiMode Nanoscope IIIa (Digital Instruments, USA). The device is equipped with a J scanner, which was calibrated using the manufacturer's grating. Ultrasharp tips (Noncontact "Golden" Silicon cantilevers, NSG10S, typical force constant 11.5 N/m, resonant frequency 255 kHz) were used. Height images are flattened to remove background slopes. No other filtering procedures are performed on these images.
Static SIMS images were acquired with a TOF-SIMS IV (ION-TOF), using a pulsed Bi+ primary ion beam (burst alignment mode, 25 KeV, 0.5 pA, 100 μm × 100 μm raster, PI fluence < 3 × 1011 ions/cm2). Detailed images were obtained from small areas (100 μm × 100 μm with 256 × 256 pixel definition) using the high spatial imaging mode. This allows a spatial resolution of about 200 nm; however, mass resolution is greatly degraded. Analyses below the static limit were performed.
Results and discussion
In particular, the appearance of a well-defined plateau region around a surface pressure of 17 mN/m for the concentration of 5 mg/ml is diagnostic of the formation of the liquid/solid-like region characteristic of the circular domains. Accordingly, the 5 mg/ml concentration corresponds to the critical micellar concentration (CMC) for the specific Pn BuA-b-PAA employed in this study .
Therefore, in order to obtain a well-packed Pn BuA-b-PAA film, the deposition was performed well above the plateau surface pressure, i.e., at a surface pressure of 25 mN/m. According to wide literature, the structure of the film in the solid-like phase region is the result of drastic self-assembling processes of the different polymer blocks, basically yielding circular domains based on PAA chains, protruded towards the water subphase, and a matrix based on Pn BuA chains, spread at the water/air interface. The transfer of the films onto solid surfaces (silicon) by HP-LB method maintains the lateral inhomogeneity of the film structure [31, 34, 35].
Figure 2b shows the effect of the Au sputtering deposition. One can observe the decrease of the height of the hydrophilic PAA-based circular domains with respect to the matrix in the height image, whilst in the phase image, as expected for the homogeneous Au NP coating produced, one can observe a uniform and unstructured image, corresponding to the perfectly homogeneous coating of Au.
By AFM characterization of the annealed bilayer (Figure 2c) we have again evidenced of a phase separation. The nanoparticles' distribution onto the block copolymer domains, studied by AFM, seems strongly affected by the bilayer annealing, showing an apparent return of the initial dephasing of the HP-LB block copolymer film. Regarding the cause of this return of the dephasing we can do some hypothesis: (1) Gold segregation onto the polar domains because of the increased diffusion of gold onto diblock copolymer film during the thermal annealing (higher mobility of gold  because of the higher fluidity of polymer chains) and furthermore due to new positioning of gold driven by block copolymer template. (2) The second hypothesis is an in-depth diffusion of gold as Kunz et al.  have just observed for discontinuous gold films on amorphous polymer substrates. In fact amorphous polymers behave as viscous fluids at temperatures above glass transition temperatures and such behaviour could induce an increasing of the mobility of gold. (3) Third hypothesis implies a modification of the surface-tip interaction produced by new hardness or viscoelasticity properties of the uppermost layer.
with P ∞ the vapour pressure at a planar surface, γ the surface free energy of gold, Ω the atomic volume of gold, k B the Boltzmann constant, c a temperature-dependent but time-independent constant and depending on the diffusion atomic coefficient D of gold. The hypothesis 1 involves a surface diffusion of gold on block copolymer surface characterized by a surface diffusion coefficient D s. The hypothesis 2 involves, instead, a diffusion of gold into the polymer characterized by a diffusion atomic coefficient D in of gold in the polymer. Obviously, usually, D s ≫ D in. Just this purely thermodynamic consideration supports the exclusion of hypothesis 2. Nevertheless, for example Kunz  observed an in-depth diffusion of gold in polystyrene after annealing. Therefore, we performed the step-by-step TOF-SIMS imaging in order to exclude experimentally and directly the first and the second hypotheses.
We have investigated all the three different steps: (1) HPLB film, (2) hybrid bilayer AuNPs/BCs, (3) annealed hybrid bilayer.
In Figure 4a we observe the results of separation phase phenomena and the presence of circular domains in HP-LB film of Pn BuA-b-PAA (Figure 4a). In particular, the bidimensional distributions of the normalized intensities of some molecular fragments (m/z: 28, 29, 41, 42, 57 and 197 Da that correspond to CO+, CHO+, C2HO+, C2H2O+, C4H9 + and Au+, respectively) are shown and the complementarity between PAA molecular fragments (m/z: 28, 57 Da) and Pn BuA molecular fragments (m/z: 29, 41, 42 Da). After gold sputtering deposition we observe the annealing of inhomogeneous composition of the film and the homogeneous surface distribution of gold ion (Figure 4b). Finally, also in Figure 4c the homogeneous distributions of all of the fragments are shown.
In summary, TOF-SIMS imaging allows us to exclude again the first hypothesis, as we know because of the experimental evidence shown in the graphic of Figure 3, but allows us to exclude also the second hypothesis (regarding the in depth diffusion of gold) because we have no evidence by SIMS imaging of gold depletion phenomenon and its diffusion under block copolymer film, in fact we observe an homogeneous distribution of molecular fragments in the uppermost layer after annealing (Figure 4c).
By means of the comparison of the nanometric scale morphology before and after the thermal annealing (Figure 5b,c) we observe the nanostructures modification induced by annealing. The new morphology of gold nanostructures is apparently independent on the morphology at the nanoscale of the block copolymer film as we can deduce by the comparison of Figure 5a and 5c.
In summary, hybrid bilayer exhibits a memory effect induced by thermal annealing and these effects can be explained by third hypothesis that takes into account only a modified surface-tip interaction induced by thermal annealing. Such hypothesis is supported by the comparison of the nanometric scale morphologies of the block copolymer film, of hybrid bilayer and annealed hybrid bilayer shown in the AFM images of Figure 5. In fact, after thermal annealing, above T g temperatures, of both of the blocks, the uppermost modified nanostructured gold layer (shown in Figure 5c), become sensitive to the immediately underlying block copolymer film, probably due to the increased diffusion of gold onto diblock copolymer film during the annealing (higher mobility of polymer chains). When gold atoms are sputter-deposited at room temperature onto insulator substrates they, generally, grow in the Volmer-Weber mode forming three-dimensional clusters [39, 40]. It is a consequence of the fact that the surface free energy of gold (1.5 J/m2) is higher than that one of the insulator substrates (typically in the range 10-100 mJ/m2). In general, this growth mode for gold on polymers surfaces also occurs (for example the surface energy of Pn BuA is about 37 mJ/m2) [37, 41–43]. As a consequence, a low adhesion energy (E d) for the gold on polymer substrates is obtained (with respect to gold deposited on metallic or semiconductor substrates). Thermal annealing determines a modification of surface morphology of the gold nanostructures and an increase of the adhesion energy of the gold with Pn BuA block (E d1) and with pAA block (E d2). The different values of E d1 and E d2 determine the interaction modification of the tip with gold on circular domains (constituted by block 1 PAA) and with gold on the remaining matrix (constituted by Pn BuA) resulting in the return of two different phases.
The organization of metallic nanoparticles within polymer films can be achieved using many routes. Our method exploits the self-organization characteristic of sputtered Au nanoparticles on self-assembled Pn BuA-b-PAA film obtained by HP-LB method. We studied the morphology and the phase-separation of the film before and after Au sputtering. The effect of the increased mobility of the polymer chains onto the nanoparticles' organization has been studied by heating the polymer-Au bilayer at T >T g.
The nanoparticles' distribution onto the block copolymer domains, studied by AFM and TOF-SIMS, seems strongly affected by the bilayer annealing. In particular, hybrid bilayers exhibit memory effects as a consequence of thermal annealing. Such effects are proved by morphological and compositional experimental evidence of Au NPS/Block copolymer hybrid bilayer and can be explained by the hypothesis that takes into account a modified surface-tip interaction induced by thermal annealing. Such hypothesis is supported by the comparison of the nanomorphologies of the block copolymer film, of hybrid bilayer and annealed hybrid bilayer shown in the AFM images. In fact, after thermal annealing, above T g temperatures of both of the blocks, the uppermost modified nanostructured gold layer becomes sensitive to the immediately underlying block copolymer film, probably due to the increased diffusion of gold onto diblock copolymer film during the annealing. In particular, thermal annealing determines a modification of surface morphology of the gold nanostructures and an increase of the adhesion energy of the gold with Pn BuA block (E d1) and with PAA block (E d2). The different values of E d1 and E d2 determine the interaction modification of the tip with gold on circular domains (constituted by block 1 PAA) and with gold on the remaining matrix (constituted by Pn BuA) resulting in the return of two different phases. Furthermore, annealing at T >T g does not induce polymer mixing between two blocks or between blocks and gold.
atomic force microscopy
critical micellar concentration
horizontal precipitation Langmuir-Blodgett
- Pn BuA-b-PAA poly-n :
time of flight secondary ion mass spectrometry.
- Xia YN, Kim E, Zhao XM, Rogers JA, Prentiss M, Whitesides GM: "Complex optical surfaces formed by replica molding against elastomeric masters". Science 1996, 273: 347. 10.1126/science.273.5273.347View ArticleGoogle Scholar
- Quake SR, Scherer A: "From micro- to nanofabrication with soft materials". Science 2000, 290: 1536. 10.1126/science.290.5496.1536View ArticleGoogle Scholar
- Schmitt J, Decher G, Dressick WJ, Brandow SL, Geer RE, Shashidhar R, Calvert JM: "Metal nanoparticle/polymer superlattice films: Fabrication and control of layer structure". Adv Mater 1997, 9: 61. 10.1002/adma.19970090114View ArticleGoogle Scholar
- Krishnan RS, Mackay ME, Duxbury PM, Pastor A, Hawker CJ, Van Horn B, Asokan S, Wong MS: "Self-assembled multilayers of nanocomponents". Nano Lett 2007, 7: 484. 10.1021/nl062866uView ArticleGoogle Scholar
- Tjandra W, Yao J, Ravi P, Tam KC, Alamsjah A: "Nanotemplating of calcium phosphate using a double-hydrophilic block copolymer". Chem Mater 2005, 17: 4865. 10.1021/cm050679bView ArticleGoogle Scholar
- Thurn-Albrecht T, Schotter J, Kastle CA, Emley N, Shibauchi T, Krusin-Elbaum L, Guarini K, Black CT, Tuominen MT, Russell TP: "Ultrahigh-density nanowire arrays grown in self-assembled diblock copolymer templates". Science 2000, 290: 2126. 10.1126/science.290.5499.2126View ArticleGoogle Scholar
- Lu JQ, Yi SS: "Uniformly sized gold nanoparticles derived from PS-b-P2VP block copolymer templates for the controllable synthesis of Si nanowires". Langmuir 2006, 22: 3951. 10.1021/la053377xView ArticleGoogle Scholar
- Minelli C, Hinderling C, Heinzelmann H, Pugin R, Liley M: "Micrometer-long gold nanowires fabricated using block copolymer templates". Langmuir 2005, 21: 7080. 10.1021/la050757+View ArticleGoogle Scholar
- Horiuchi S, Fujita T, Hayakawa T, Nakao Y: "Three-dimensional nanoscale alignment of metal nanoparticles using block copolymer films as nanoreactors". Langmuir 2003, 19: 2963. 10.1021/la020745dView ArticleGoogle Scholar
- Adachi M, Okumura A, Sivaniah E, Hashimoto T: "Incorporation of metal nanoparticles into a double gyroid network texture". Macromolecules 2006, 39: 7352. 10.1021/ma061108nView ArticleGoogle Scholar
- Black CT, Murray CB, Sandstrom RL, Sun SH: "Spin-dependent tunneling in self-assembled cobalt-nanocrystal superlattices". Science 2000, 290: 1131. 10.1126/science.290.5494.1131View ArticleGoogle Scholar
- Sanchez C, Julian B, Belleville P, Popall M: "Applications of hybrid organic-inorganic nanocomposites". J Mater Chem 2005, 15: 3559. 10.1039/b509097kView ArticleGoogle Scholar
- Sanchez C, Lebeau B: "Design and properties of hybrid organic-inorganic nanocomposites for photonics". MRS Bull 2001, 26: 377. 10.1557/mrs2001.91View ArticleGoogle Scholar
- Roth SV, Walter H, Burghammer M, Riekel C, Lengeler B, Schroer C, Kuhlmann M, Walther T, Sehrbrock A, Domnick R, Müller-Buschbaum P: "Combinatorial investigation of the isolated nanoparticle to coalescent layer transition in a gradient sputtered gold nanoparticle layer on top of polystyrene". Appl Phys Lett 2006, 88: 021910. 10.1063/1.2161926View ArticleGoogle Scholar
- Takele H, Schurmann U, Greve H, Paretkar D, Zaporojtchenko V, Faupel F: "Controlled growth of Au nanoparticles in co-evaporated metal/polymer composite films and their optical and electrical properties". Eur Phys J Appl Phys 2006, 33: 83. 10.1051/epjap:2006006View ArticleGoogle Scholar
- Biswas A, Marton Z, Kanzow J, Kruse J, Zaporojtchenko V, Faupel F, Strunskus T: "Controlled generation of Ni nanoparticles in the capping layers of Teflon AF by vapor-phase tandem evaporation". Nano Lett 2003, 3: 69. 10.1021/nl020228fView ArticleGoogle Scholar
- Biswas A, Aktas OC, Kanzow J, Saeed U, Strunskus T, Zaporojtchenko V, Faupel F: "Polymer-metal optical nanocomposites with tunable particle plasmon resonance prepared by vapor phase co-deposition". Mater Lett 2004, 58: 1530. 10.1016/j.matlet.2003.10.037View ArticleGoogle Scholar
- Kay E: "Synthesis and properties of metal-clusters in polymeric matrices". Z Phys D 1986, 3: 251. 10.1007/BF01384814View ArticleGoogle Scholar
- Lauter-Pasyuk V, Lauter HJ, Ausserre D, Gallot Y, Cabuil V, Hamdoun B, Kornilov EI: "Neutron reflectivity studies of composite nanoparticle copolymer thin films". Phys B 1998, 248: 243. 10.1016/S0921-4526(98)00241-5View ArticleGoogle Scholar
- Lin Y, Boker A, He JB, Sill K, Xiang HQ, Abetz C, Li XF, Wang J, Emrick T, Long S, Wang Q, Balazs A, Russell TP: "Self-directed self-assembly of nanoparticle/copolymer mixtures". Nature 2005, 434: 55. 10.1038/nature03310View ArticleGoogle Scholar
- Hamdoun B, Ausserre D, Joly S, Gallot Y, Cabuil V, Clinard C: "New nanocomposite materials". J Phys II 1996, 6: 493. 10.1051/jp2:1996106Google Scholar
- Lauter-Pasyuk V, Lauter HJ, Gordeev GP, Müller-Buschbaum P, Toperverg BP, Jernenkov M, Petry W: "Nanoparticles in block-copolymer films studied by specular and off-specular neutron scattering". Langmuir 2003, 19: 7783. 10.1021/la026818aView ArticleGoogle Scholar
- Frömsdorf A, Kornowski A, Putter S, Stillrich H, Lee LT: "Highly ordered nanostructured surfaces obtained with silica-filled diblock-copolymer micelles as templates". Small 2007, 3: 880.View ArticleGoogle Scholar
- Hashimoto T, Harada M, Sakamoto N: "Incorporation of metal nanoparticles into block copolymer nanodomains via in-situ reduction of metal ions in microdomain space". Macromolecules 1999, 32: 6867. 10.1021/ma990378lView ArticleGoogle Scholar
- Jain A, Hall LM, Garcia CBW, Gruner SM, Wiesner U: "Flow-induced alignment of block copolymer-sol nanoparticle coassemblies toward oriented bulk polymer-silica hybrids". Macromolecules 2005, 38: 10095. 10.1021/ma0483930View ArticleGoogle Scholar
- Abul Kashem MMA, Perlich J, Schulz L, Roth SV, Petry W, Müller-Buschbaum P: "Maghemite nanoparticles on supported diblock copolymer nanostructures". Macromolecules 2007, 40: 5075. 10.1021/ma070782hView ArticleGoogle Scholar
- Barnes KA, Karim A, Douglas JF, Nakatani AI, Gruell H, Amis EJ: "Suppression of dewetting in nanoparticle-filled polymer films". Macromolecules 2000, 33: 4177. 10.1021/ma990614sView ArticleGoogle Scholar
- Barnes KA, Douglas JF, Liu DW, Karim A: "Influence of nanoparticles and polymer branching on the dewetting of polymer films". Adv Colloid Interface Sci 2001, 94: 83. 10.1016/S0001-8686(01)00056-2View ArticleGoogle Scholar
- Krishnan RS, Mackay ME, Duxbury PM, Hawker CJ, Asokan S, Wong MS, Goyette R, Thiyagarajan P: "Improved polymer thin-film wetting behavior through nanoparticle segregation to interfaces". J Phys: Condens Matter 2007, 19: 356003. 10.1088/0953-8984/19/35/356003Google Scholar
- Lopes WA: "Nonequilibrium self-assembly of metals on diblock copolymer templates". Phys Rev E 2002, 65: 031606. 10.1103/PhysRevE.65.031606View ArticleGoogle Scholar
- Zhavnerko GK, Staroverov VN, Agabekov VE, Gallyamov MO, Yaminsky IV: "Interpretation of SPM images of Langmuir-Blodgett films based on long-chain carboxylic acids". Thin Solid Films 2000, 359: 98. 10.1016/S0040-6090(99)00734-8View ArticleGoogle Scholar
- Li S, Hanley S, Khan I, Varshney SK, Eisenberg A, Lennox RB: "Surface micelle formation at the air-water-interface from non-ionic diblock copolymers". Langmuir 1993, 9: 2243. 10.1021/la00032a057View ArticleGoogle Scholar
- Eghbali E, Colombani O, Drechsler M, Axel HE, Müller AHE, Hoffmann H: "Rheology and phase behavior of poly(n-butyl acrylate)-block-poly(acrylic acid) in aqueous solution". Langmuir 2006, 22: 4766. 10.1021/la053272uView ArticleGoogle Scholar
- Torrisi V, Tuccitto N, Delfanti I, Audinot JN, Zhavnerko GK, Migeon HN, Licciardello A: "Nano- and microstructured polymer LB layers: A combined AFM/SIMS study". Appl Surf Sci 2008, 255: 1006. 10.1016/j.apsusc.2008.05.098View ArticleGoogle Scholar
- Torrisi V, Licciardello A, Marletta G: "Chemical imaging of self-assembling structures in Langmuir-Blodgett films of polymer blends". Mater Sci Eng B 2010, 169: 49. 10.1016/j.mseb.2009.12.004View ArticleGoogle Scholar
- Ruffino F, Torrisi V, Marletta G, Grimaldi MG: "Kinetic growth mechanisms of sputter-deposited Au films on mica: from nanoclusters to nanostructured microclusters". Appl Phys A 2010, 100: 7. 10.1007/s00339-010-5797-7View ArticleGoogle Scholar
- Kunz MS, Shull KR, Kellock AJ: "Morphologies of discontinuous gold-films on amorphous polymer substrates". J Appl Phys 1992, 72: 4458. 10.1063/1.352362View ArticleGoogle Scholar
- Tu KN, Mayer JW, Feldman LC: Electronic Thin Film Science. New York: Macmillan Publishing Company; 1992.Google Scholar
- Campbell CT: "Ultrathin metal films and particles on oxide surfaces: Structural, electronic and chemisorptive properties". Surf Sci Rep 1997, 27: 1. 10.1016/S0167-5729(96)00011-8View ArticleGoogle Scholar
- Venables JA, Spiller GDT, Hanbüken M: "Nucleation and Growth of thin films". Rep Prog Phys 1984, 47: 399. 10.1088/0034-4885/47/4/002View ArticleGoogle Scholar
- Smithson RLW, McClure DJ, Evans DF: "Effects of polymer substrate surface energy on nucleation and growth of evaporated gold films". Thin Solid Films 1997, 307: 110. 10.1016/S0040-6090(97)00310-6View ArticleGoogle Scholar
- Kaune G, Ruderer MA, Metwalli E, Wang W, Couet S, Schlage K, Röhlsberger R, Roth SV, Müller-Buschbaum P: "In Situ GISAXS Study of Gold Film Growth on Conducting Polymer Films". Appl Mater Interfaces 2009, 1: 353. 10.1021/am8000727View ArticleGoogle Scholar
- Mark JE, (Ed): Physical properties of Polymers-Handbook. 2nd edition. New York: Springer; 2007:1012.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.